Investigation of Interactions between Liquid Iron …9456/FULLTEXT01.pdf · Investigation of...
Embed Size (px)
Transcript of Investigation of Interactions between Liquid Iron …9456/FULLTEXT01.pdf · Investigation of...
Investigation of Interactions between Liquid Iron Containing Oxygen and Aluminosilicate Refractories
Department of Material Science and Engineering Division of Metallurgy
Royal Institute of Technology SE-100 44 Stockholm
Akademisk avhandling som med tillstnd av Kungliga Tekniska Hgskolan i Stockholm, framlgges fr offentlig granskning fr avlggande av Teknologie doktorsexamen, fredagen den 31 oktober 2003, kl. 10.00 i Kollegiesalen, Administrationsbyggnaden, KTH, Valhallavgen 79, Stockholm
ABSTRACT The present work was initiated to investigate runner refractory corrosion by molten steel. The aim was to understand the mechanism of inclusion formation during ingot casting. The work is also of interest to other unit processes in steel making, where refractory corrosion and erosion are serious problems. The oxides investigated in the present work were alumina, silica and mullite, which are the main components in runner refractory. In addition, industrial refractory material was investigated. Two types of experiments were conducted. The first, rod experiments, involved dipping a rod of the oxide into an iron bath containing varying amounts of oxygen. After quenching, the rods were examined through SEM/EDS analysis. In the second sets of experiments, the wetting behaviour of molten iron on refractory oxides was investigated by means of the sessile-drop method. The reactions were followed in static as well as dynamic modes through contact angle measurements. Temperature and oxygen partial pressure were, besides time the parameters that were investigated in the present study. Oxygen partial pressure was defined by introducing a gas mixture of CO-CO2-Ar into the furnace. The experimental studies were preceded by a thermodynamic investigation of the refractory systems, in order to get a fundamental understanding of the reactions that occurred. Phase stability diagrams for the systems were constructed based on the data available in literature. The diagrams showed that the reaction between alumina and oxygen containing iron would lead to the formation of hercynite at a critical oxygen level in the metal. With silica, the reaction would lead to the formation of fayalite. In the mullite case, the reaction products would be hercynite at moderate oxygen levels in the melt and hercynite together with fayalite at slightly higher oxygen potentials. For all substrates, the contact angles started decreasing as the surface-active oxygen came into contact with the iron drop. At a critical level of oxygen in the metal, a reaction product started forming at the drop/substrate interface. The reaction products were identified through SEM/EDS analysis and were found to be in agreement with thermodynamic predictions. In the case of SiO2 substrate, there were also deep erosion tracks along the periphery of the drops, probably due to Marangoni flow. Alumina-graphite refractory reactions with molten iron were also investigated through Monte Carlo simulations. The results showed that, with increased alumina content in the refractory, the carbon dissolution into the melt decreased. Further, the wetting behaviour at the interface was found to be an important factor to considerably reduce the carbon dissolution from alumina-graphite refractories. The experimentation was extended to the commercial refractories used in the ingot casting process at Uddeholm Tooling AB, Sweden. The analysis of the plant trial samples indicates that there is less likelihood of a strong corrosion of the refractories that could lead to a significant population of inclusions in the end product. The impact of the present experimental results on refractory erosion is discussed. The importance of the results to clean steel processing and development of new generation refractories are also presented.
Aum Shri Ganeshaya namah
ACKNOWLEDGEMENTS First, and most of all, I would like to thank my supervisor and guru Professor Seshadri Seetharaman. You demanded hard work, 25 hours a day, 8 days a week. Still, I cannot, in words express what your support and belief in me has meant. I am indebted to Associate Professor Veena Sahajwalla, for giving me the opportunity to work with her at The University of New South Wales, Sydney, Australia. I am also grateful to Professor Ashok K. Lahiri for his valuable suggestions and constructive criticism. I would like to thank Professor Pr Jnsson for giving me the opportunity to work with this project. Professor Du Sichen is acknowledged for helpful comments and suggestions. Financial support from Brinell Centre for this project is gratefully acknowledged. So are the help and comments from Alf Sandberg, Uddeholm Tooling AB. Hans Bergqvist, KTH, and Lena Eliasson, Uddeholm Tooling AB, are thanked for helping me understand the complicated world of SEM. Peter Kling acted valiantly whenever experimental equipment had to be beaten/conquered/fought and is therefore acknowledged. Colleagues and friends at the Division of Metallurgy are acknowledged for their camaraderie. Friends and colleagues at UNSW are fondly remembered for making my year in Sydney unforgettable. Special thanks are due to Andrea Al-Badri, Gregory Perkins, Tsuey Cham, Brian Mubaraki and Raymond Longbottom; I really enjoyed your company. Fredrik Nyman is acknowledged for constant support, help and understanding. Abha Kapilashrami, my dearest sister and personal advisor, for moral support, encouragement and good advice. This thesis is dedicated to my parents, Chakra Dhar and Bina Kapilashrami, for their love and pride in me. Era Kapilashrami Stockholm September 2003
SUPPLEMENTS This thesis is based on the following papers: Supplement 1: Corrosion of dense alumina by molten iron containing
oxygen: E. Kapilashrami, A.K. Lahiri and S. Seetharaman.
Steel Grips 1, 2003, No. 2, pp. 126-132. Supplement 2: Studies of the Wetting Characteristics of Liquid Iron on Dense
Alumina by the X-Ray Sessile Drop Technique: E. Kapilashrami, A. Jakobsson, A.K. Lahiri and S. Seetharaman.
Metall. Mater. Trans. B, 2003, vol. 34B, pp. 193-199.
Supplement 3: Investigation of the Reaction between Oxygen-Containing
iron and SiO2 Substrate by X-Ray Sessile-Drop Technique: E. Kapilashrami, A.K. Lahiri. A.W. Cramb and S. Seetharaman.
Metall. Mater. Trans B, 2003, in press
Supplement 4: Investigation of the Wetting Characteristics of Liquid Iron on
Mullite by Sessile Drop Technique: E. Kapilashrami, V. Sahajwalla and S. Seetharaman.
Accepted for publication in ISIJ International, September 2003 Supplement 5: Carbon Dissolution from Graphite-Alumina Refractory
Mixtures into Liquid Iron: A Monte Carlo Simulation Study: V. Sahajwalla, R. Khanna, E. Kapilashrami and S. Seetharaman.
Sent to Metall. Mater. Trans. B for publication, August 2003 Supplement 6: Reactions between Runner Refractory and Molten Steel
during Casting Practice at Uddeholm Tooling AB: E. Kapilashrami, H. Issal and A. Sandberg.
The authors contribution to the different supplements of this thesis: Supplement 1: Literature survey, thermodynamic evaluation, experimental
work, microscopic evaluation and part of the writing. Approximate contribution: 75%.
Supplement 2: Literature survey, experimental work, microscopic evaluation
and part of the writing. Approximate contribution: 75%. Supplement 3: Literature survey, thermodynamic evaluation, experimental
work, microscopic evaluation and major part of the writing. Approximate contribution: 80%.
Supplement 4: Literature survey, thermodynamic evaluation, experimental
work, microscopic evaluation and major part of the writing. Approximate contribution: 85%.
Supplement 5: Literature survey. Approximate contribution 20%. Supplement 6: Experimental work, microscopic evaluation and major part of
the writing. Approximate contribution: 90%
Parts of the work have also been presented at the following conferences:
I. Reactions between Molten Iron and Lining Materials: E. Kapilashrami, P. Jnsson and S. Seetharaman
Poster presentation at the 6th International Conference of Molten Slags, Fluxes and Salts, Stockholm, Sweden-Helsinki, Finland, 12-17 June, 2000
II. Reactions Between Refractories and Molten Iron in Steelmaking Processes: E. Kapilashrami, A. Jakobsson and S. Seetharaman
Presented at the 59th Electric Furnace Conference, Phoenix, Arizona, USA, 11-14 November, 2001.
III. Static and Dynamic Thermophysical property Measurement at High
Temperatures S. Seetharaman, S. Du, R. Eriksson and E. Kapilashrami.
Presented at Mills symposium, London, UK, 22-23 August 2002 and accepted for publication in High Temperature Materials and Processes. (Included as Appendix A)
Parts of the work have been accepted for presentation in the following conferences:
IV. Slag formation during High-Temperature interactions between SiO2containing Refractories and Iron Melts with Oxygen E. Kapilashrami, V. Sahajwalla and S. Seetharaman.
Accepted for presentation in International conference on Molten Slags Fluxes and Salts, Cape Town, South Africa, 25-28 January 2004. (Included as Appendix B)
V. Wetting Characteristics of Oxygen-Containing Iron melts on refractory
oxides: E. Kapilashrami and S. Seetharaman.
Accepted for presentation in Fourth International Conference High Temperature Capillarity, HTC 2004, Sanremo-Genoa, Italy March 31-April 3 2004.
TABLE OF CONTENTS
1. INTRODUCTION 1
2. THEORETICAL ASPECTS 3
2.1 Thermodynamic investigation of the systems 3 2.1.1 Thermodynamic analysis of the Fe-O-Al system 3 2.1.2 Thermodynamic analysis of the Fe-O-Si system 4 2.1.3 Thermodynamic analysis of the Fe-O-Al-Si system 5
2.2 Surface reactions 7
3. EXPERIMENTAL METHODS 9
3.1 Rod experiments 9 3.2 Sessile-drop experiments 9
4. RESULTS 11 4.1 Rod experiments 11 4.2 Sessile-drop experiments 12
4.2.1 Iron on alumina substrate 12 4.2.2 Iron on silica substrate 14 4.2.3 Iron on mullite substrate 16
5. INDUSTRIAL REFRACTORY MATERIAL 19
6. MONTE CARLO SIMULATIONS 21 6.1 Theoretical model 21 6.2 Results 21
7. DISCUSSION 23
8. CONCLUSIONS 29
8. FUTURE WORK 31
9. REFERENCES 33
Refractories are ceramics consisting of chemically stable, non-metallic compounds or mixtures of the same. Their heat resistance and hardness make them suitable for lining purpose in steelmaking vessels. However, conditions prevailing under steelmaking processes are aggressive, making the ceramics susceptible to corrosion. This, together with their brittle nature, poses limitation to their applicability. The stability of the refractories depends on the strength and porosity of the refractory material. Refractory wear in steelmaking processes creates serious problems, with implications on process economy and environment. Fundamental knowledge of the mechanisms of refractory wear caused by liquid steel and slags is considered very important in the economic optimisation of steelmaking processes. In addition, refractory erosion by molten steel during the refining and casting steps of the process can contribute to the formation of non-metallic inclusions in steel, resulting in an adverse effect on the steel quality. In the ingot processing of steel, the molten metal flows through refractory runners into the ingot. The refractory in the runners comes under severe attack by the molten steel. This attack consists of two parts, viz. the chemical corrosion as well as the mechanical erosion wherein the refractory is peeled off and the pieces follow the flowing metal. Corrosion and erosion of runner refractories can lead to accumulation of oxide inclusions in the steel, resulting in the formation of micro- and macro inclusions, leading to the downgrading of the steel quality in terms of steel cleanliness. The resistance to chemical corrosion of the refractory materials can be improved by choosing materials of better thermodynamic stability or by generating kinetic/diffusion barriers that hinder the propagation of the corrosion reaction. These areas require fundamental understanding of both thermodynamics and kinetics, including mass transfer aspects, of the reactions involved. Another important aspect calling for increased attention is the extent of the surface reactions. The present project was initiated with an aim to investigate the corrosion reactions in uphill teeming of steel during ingot casting, with a special focus on runner refractories. The objective was to develop a fundamental understanding of the mechanism involved so that industrial practice could be optimised by further improvements by the choice of refractories. Molten steel contains a number of dissolved elements including carbon, oxygen and sulphur in very small quantities. Earlier work1,2 showed that reactions between FeO in slags and refractory linings have a serious impact on the corrosion of the refractories. Hence, it was felt that reactions between oxygen-containing iron and the refractory lining could be of utmost importance. The runner refractory used in the steel industry mainly consists of Al2O3 and SiO2. Examination of the phase diagram3 of the system Al2O3-SiO2 reveals the formation of the stable compound, mullite with the formula 3 232 2SiOOAl . The Gibbs energy of formation for this compound is low4, ca 30 kJmole-1 at 1873 K; hence it is reasonable to assume that it could be the predominant phase in runner refractory. The present work was therefore planned in accordance with the scheme in Figure 1. To
gain a sound comprehension of the phenomenon involving molten iron and refractory reactions, it is crucial to understand how the different oxides reacted individually with iron.
molten iron-Al2O3 molten iron-SiO2
molten iron-mullite 3Al2O22SiO2
Figure 1. A schematic figure of the structure of the present study, the reactions between molten iron
and different oxides An investigation of the reactions between pure liquid iron containing varying amounts of oxygen and alumina as well as silica was therefore carried out before mullite and industrial refractory substrate were investigated. The information obtained is intended to serve as a foundation for industrial refractory practice. Macro and micro scale experiments were designed to investigate the reactions between molten iron and solid oxides. The macro scale experiments gave a general idea of the reaction between molten and solid phase. In these experiments, dense rods of the oxides were dipped into molten iron containing varying amounts of oxygen. The reactions on micro scale were performed to investigate the surface reaction of molten iron on oxides. This was carried out through sessile-drop experiments, and the reactions were followed statically as well as dynamically. Investigations of the reaction between alumina-containing refractory and molten iron, on an atomic level were also carried out through Monte Carlo simulations. The refractory simulated consisted of varying amounts of alumina and graphite. The reaction rate was measured through carbon dissolution into the molten iron. The simulations were expected to give a deeper knowledge of refractory-molten metal reactions.
2. THEORETICAL ASPECTS
2.1 Thermodynamic investigation of the systems To understand the stability of the phases formed during the above-discussed reactions, thermodynamic analyses of the different systems, Fe-O-Al, Fe-O-Si and Fe-O-Al-Si were carried out. Input data from literature for the systems were critically assessed and compared, the results of which are shown in Table I. The data were then used to construct a phase stability diagram. Table I. Comparison between different input data for Gibbs energy of formation for hercynit, fayalite and mullite respectively.
Reference Gibbs energy of formation, G [Jmole-1]
)(42)(2)(32)( 2/1 sgsl OFeAlOOAlFe =++
Barin4 G=-328,348+82.044T Chan, Alcock and Jacob5 G=-306,248+76.316T McLean and Ward6 G=-267,399+52.467T Richardson, Jeffes and Withers7 G=-313,800+87.446T Pillay, DEntremont and Chipman8 G=-246,250+43.750T* Thermocalc9 G=-309,954+75.683T
)(42)(22)(2 lsl SiOFeSiOOFe =++
Barin4 G=-518,959+116.82T Knacke, Kubaschewski and Hasselmann10 G=-627,695+196.414T Thermocalc9 G=-474,242+82.476T
)(232)(2)(32 2323 sss SiOOAlSiOOAl =+
Barin4 G=18,779-26.953T Turkdogan11 G=8,593-17.405T Rein and Chipman12 G=-4,861-16.119T* *Estimated from R. Yamanaka, S. Koyama and M. Iwase, Metall. Met. Trans. B, 1991, vol. 22B, pp. 839 As seen, there is a slight discrepancy between the reported values. For the sake of consistency only the values from Barin4 are used in the following calculations. 2.1.1 Thermodynamic analysis of the Fe-O-Al system The phase diagram for the system FeO-Al2O313 shows the existence of one intermediate compound, viz. FeAl2O4 (hercynite). The reaction and its Gibbs energy of formation for solid hercynite4, are according to Equation 1:
sgsl OFeAlOOAlFe =++ (1)
TG += 044.82348,32801 Jmole
-1 [T range 1809 K and above] The activities of alumina, iron and hercynite are assumed to be 1 and the interactions from dissolved aluminium and oxygen are neglected. From the values, a phase
stability diagram was constructed with temperature as a function of partial pressure of oxygen in the system Fe-O-Al. The diagram is presented in Figure 2:
PO2 [Pa] Figure 2. The phase stability diagram for the system Fe-O-Al. Mutual solubility between Al2O3 and
FeAl2O4 is not considered At slightly higher oxygen levels, solid FeAl2O4 will exist up to approximately 2053 K, thereby implying that, under suitable conditions, FeAl2O4 is likely to form. The present analysis does not consider any possible solid solution formation between Al2O3 and FeAl2O4. 2.1.2 Thermodynamic analysis of the Fe-O-Si system In the case of silica, as the substrate comes in contact with liquid iron containing oxygen, the calculations show that two silicates are likely to form in the system, i.e. orthosilicate and metasilicate. For orthosilicate (fayalite), the reaction, and its Gibbs energy of formation, are as follows:
)(42)(22)(2 lsl SiOFeSiOOFe =++ (2)
T82.161518,959 -02 +=G Jmole-1 [T range 1490- 1700 K]
The corresponding value for formation of metasilicate is
)(32)(2)( )(21 sgl FeSiOsSiOOFe =++ (3)
T32.123352,361 03 +=G Jmole-1 [T range up to 1400 K]
In the calculations, activities of silica, iron and fayalite are assumed to be 1 and the interactions from dissolved silicon and oxygen are neglected. At steelmaking temperatures, only the orthosilicate (fayalite) in liquid form will be the stable phase. However, as the system is cooled down, metasilicate can precipitate. The Gibbs energy of formation for fayalite, extrapolated from the reported values by Barin4 was
used to construct a phase stability diagram for the system. The diagram is presented in Figure 3:
PO2 [Pa] Figure 3. Phase stability diagram constructed for the system Fe-O-Si with extrapoleted data from
Barin4. Mutual souluility between SiO2 and Fe2SiO4 has not been considered. The constructed phase stability diagram shows that Fe2SiO4 will form if the oxygen partial pressure in the gas exceeds 310-4 Pa at 1850 K. This is likely to happen during certain steelmaking steps where the oxygen potential in the slag is high. In reality, the reactions will occur through oxygen dissolved in molten iron. The reaction for fayalite formation and the Gibbs energy of formation would be:
)(42)(2)()( 22 lsFel SiOFeSiOOFe =++ (4)
T59.221284,655 -04 +=G Jmole-1 [T range up to 1700 K]
Correspondingly, for metasilicate formation:
)(3)(2)()( ssFel FeSiOSiOOFe =++ (5)
T126.21235,209 05 +=G Jmole-1 [T range up to 1400 K]
2.1.3 Thermodynamic analysis of the Fe-O-Al-Si system In the aluminosilicate (mullite) case, the phase stability diagram was constructed for the quaternary system Fe-Al-Si-O and is presented in Figure 4. The reactions involved in the stability diagram calculations are:
)(2)(3)(232/3)(3 2422322 sSiOsOFeAlsSiOOAlOlFe +=++ (6)
)(2)(3)(232/7)(7 42422322 lSiOFesOFeAlsSiOOAlOlFe +=++ (7)
FeAl2O4(s) + Fe2SiO4(l)
Hercynite + SiO2 Hercynite + Fayelite
Figure 4. Phase stability diagram for the system Fe-O-Al-Si. Mutual solubility between compounds has
not been considered. At 1850 K and very low oxygen partial pressures in the gas, i.e. approximately 210-5 Pa, mullite will be stable in contact with Fe. At slightly higher oxygen content in the gas, i.e. 410-5 Pa at the same temperature, mullite reacts with the oxygen-containing iron to form hercynite and SiO2 both in solid state. The diagram also shows that fayalite, Fe2SiO4 will form along with hercynite, if the oxygen content in the gas exceeded 110-4 Pa at 1850 K. The above phase stability analysis does not consider possible solid solution formation between mullite and FeAl2O4 or solutions between fayalite and hercynite. In reality, complications arise in the quaternary system due to the dissolution of hercynite and mullite in the formed liquid fayalite. This leads to the formation of a ternary FeO-Al2O3-SiO2 slag, which will change its composition with the progress of the dissolution reaction, in accordance with the phase diagram14 presented in Figure 5.
Figure 5. Phase diagram of the system FeO-Al2O3-SiO2. The arrow points out the final slag composition in iron-oxygen-mullite system.
Furthermore, as the slag cools down, phases stable at lower temperatures (for example FeSiO3) can precipitate. Note that the formation and composition of this slag is not only dependent on the thermodynamic factors, but also on the kinetics of the reaction together with the mass-transfer aspects involved. 2.2 Surface reactions The surface tension of a metal drop can be described as the work per unit area of interface associated with splitting a liquid so that the surface molecules loose half of their neighbouring molecules15. The equilibrium drop shape is spherical. A drop in contact with either a solid or a liquid substrate will assume the shape associated with lowest possible Gibbs energy of the system. In Figure 6, a schematic figure of the forces acting on a liquid drop placed over a solid substrate is presented.
Figure 6. A schematic figure of the forces acting on a liquid drop on solid substrate
in the figure is the surface- or interfacial tension and is the contact angle in the liquid phase. For a plane and homogenous surface, the force balance involved gives the equation:
slsg = coslg (8) The surface tension of a solvent can be reduced in the presence of solutes that preferentially adsorb at the surface. Such solutes reduce the surface energy of the solvent and are named surface active elements. Wenzel16,17 investigated the effect of surface roughness on contact angle. For a rough surface, there are two areas to consider, the apparent area A , corresponding to the macroscopic dimensions of the plane and the true area , which is the area taking into account the peaks and valleys of the surface. Wenzel defined a relation between the contact angle for a smooth surface and a rough surface as:
SR r coscos = (9)
Where the subscripts R and S stand for Rough and Smooth, respectively, and r is:
Wenzels relation shows that for a wetting system, i.e. , the contact angle between a liquid and a substrate will decrease with increasing roughness. For a non-wetting area, , the contact angle will increase with increasing roughness.
090 However, Ogino et al.18 found that the difference in contact angles for smooth and rough surfaces was not pronounced for limited surface roughness, and could thus be neglected. In the present work, rough areas are assumed to be within these limits and the contact angle for the rough surface is thus assumed to be the same as for a smooth area. The dynamic change in contact angle has been investigated earlier19,20,21. Kozakevitch19 saw that the increase in mass transfer during desulphurisation of iron was accompanied by a rapid decrease in slag-metal interfacial tension. Gaye et al. 20 made similar observations. Their work also indicated that when the mass transfer decreased, the interfacial tension increased and reached its initial value. Jakobsson et al.21 saw a similar behaviour in the study of dephosphorization of iron in slag. When the dephosphorisation reaction took place, the interfacial tension and, consequently, the contact angle decreased. At the end of the dephosphorization, the interfacial tension was the same as before the reaction started.
3. EXPERIMENTAL METHODS
In the present work, two experimental methods were employed to investigate the reactions involving alumina, silica and mullite in macro- and micro scales. 3.1 Rod experiments In the macro scale experiments, the reaction between molten iron bath and the particular oxides (i.e. alumina, silica or mullite) were studied by dipping a dense rod of the oxide into the molten metal, which was kept in an argon atmosphere. The metal contained a well-defined amount of dissolved oxygen, introduced into the system by adding FeO pellets into the melt. The experimental details and the procedure adopted are presented in Supplement 1. The experiments were carried out at 1873 K with oxygen levels in molten iron corresponding to 5, 1.9 and 0.2 wt%. While 0.2 wt% oxygen in molten iron marks the saturation solubility of oxygen at the experimental temperature, the higher oxygen levels correspond to formation of free FeO in the melt. The oxygen levels were chosen to give an understanding of the corrosion mechanism when steel containing dispersed slag is reacting with refractory. Another purpose to keep the high oxygen content was to shorten the measurement time since longer treatments sometimes resulted in difficulties in keeping an inert atmosphere. The experiments were conducted over definite time intervals after which the samples were rapidly cooled. Cross sections of the rods were examined with optical microscopy and through Scanning Electron Microscopy (SEM) and Energy Dispersive Spectroscopy (EDS) analyses. 3.2 Sessile-drop experiments The second type of experiments was conducted to investigate the reaction on a micro scale. For this purpose, the sessile-drop method was used for monitoring the contact angles between molten iron and the oxide substrate at different temperatures. The changes in contact angle with time and were also investigated. These dynamic measurements were expected to provide useful information as to the reaction mechanism at micro level. The experiments were conducted, with continuously changing conditions. The surface tension of the iron drop on the substrates could therefore not be obtained and the change in contact angle was calculated instead.
The reaction sequence was followed through an image-recording device. The apparatus used and the experimental procedures are presented in Supplement 2 to 4. The oxides investigated in the present work were alumina (Supplement 2), silica (Supplement 3) and mullite (Supplement 4). Experiments were also carried out on industrial refractory (Supplement 6). The experiments took place in purified argon gas as well as in mixtures of CO, CO2 and Ar gases. To purify the gases, gas-cleaning systems were used. A schematic figure of the gas cleaning systems is shown in Figure 7.
S A flow meter
To the furnace
S: Silica gel A: Ascarite M: Magnesium perchlorate Cu: Copper turnings (823 K) Mg: Magnesium chips (773 K)
Figure 7. A schematic figure of the gas-cleaning systems used in the present work.
The moisture in the gas was removed by passing it through columns of silica gel as well as Mg(ClO4)2. CO2 was absorbed by ascarite and traces of oxygen were removed by passing the gas through copper turnings at 823 K and through magnesium chips at 773 K. The gas was then led to a gas-mixing chamber. An oxygen probe was set at the outlet of the furnace to monitor the partial pressure of oxygen in the gas. For purified argon, the oxygen probe confirmed an oxygen partial pressure Pa. 1310< The gases were led to a gas-mixing chamber, where the purified argon gas was mixed with CO and CO2 in order to get the required oxygen partial pressures used in this work. The partial pressures of oxygen obtained with the gas mixtures were
Pa, Pa and Pa as calculated by Thermocalc
4.1 Rod experiments The rod experiments were carried out to give information about reaction between lining material and molten iron on a macroscopic scale. The oxide rods were kept in an iron bath containing 0.2, 1.9 and 5 wt % oxygen for different time intervals. When the oxygen content was above the solubility limit of oxygen in molten iron, i.e. in the cases of 1.9 and 5 wt% oxygen, examination of the crucibles with solidified iron was carried out after the experiments. There were no indications that iron oxide (FeO) phase separated. The iron oxide can thus be considered completely distributed in the iron matrix. This was also confirmed by the fact that there was no preferential corrosion observed at the refractory-metal-gas interface, as floating iron oxide would preferentially attack the refractory. After rapid cooling, the rods were examined through SEM/EDS analysis. In most of the experiments, an intermediate layer was observed on the samples. The uniform thickness of the layer all around the rod indicated that the reaction was topochemical. The layer thickness was found to increase with increasing oxygen levels in the melt and with increasing treatment times. This is indicative of the prevalence of diffusion mechanism for the layer formation. The product layer seemed to have non-wetting characteristics as no metal was found to be sticking to the rods once the layer had been formed. In Figure 8, the micrograph of the cross section of the alumina rod treated in 5 wt% oxygen for 2 h is presented. Two different layers are clearly seen.
Figure 8. Micrograph of the alumina rod treated in 5 wt% oxygen for 2 h
The dark grey part corresponds to the alumina rod. The EDS analysis confirmed that this was pure Al2O3. The light grey layer in Figure 8 corresponds to the reaction product that was formed on the surface of the alumina rod. The thickness of the layer was approximately 80 m. In the experiments with 1.9 wt% oxygen, the product layer formed was much thinner and uneven. In the case of iron with 0.2 wt% oxygen, no product layer was observed.
A concentration profile of the product layer formed in Figure 8 was constructed, showing the concentrations of Al3+ and Fe2+ from EDS measurements. This is presented in Figure 9.
0 20 40 60 80 100
450 20 40 60 80 100
Al3+ Cation Fraction of Fe (at.%
Figure 9. Concentration profile of Al and Fe from EDS measurement for 5 wt% O and 2 h In the concentration profile, formation of a FeAl2O4 layer is evident. The ratio Al3+/Fe2+ shows a slight variation from the expected value of 2 for the compound FeAl2O4 indicating that the reaction product may not be stoichiometric. In the case of silica, the examination of the silica rod showed that the rod was very close to melting and completely deformed. The EDS analysis in the rod did not indicate the presence of any product layer. In the case of mullite, no results could be obtained due to experimental difficulties. The mullite rods were very brittle and disintegrated during the experiments. 4.2 Sessile-drop experiments The sessile-drop experiments were performed in the temperature range of 1823 K to 1873 K. The experiments were carried out both in purified argon as well as in CO-CO2-Ar gas mixtures. 4.2.1 Iron on alumina substrate For the experiments with iron on alumina plate, one experimental series was carried out in pure argon in the above-mentioned temperature range. Similar experiments have earlier been carried out by Jakobsson et al22, Jimbo and Cramb23, Kasama et al24, Allen and Kingery25 and Humenik and Kingery26. The contact angles measured in the present work were compared with those reported earlier for pure iron and alumina substrate and the results are presented in Figure 10.
1820 1830 1840 1850 1860
Jimbo & Cramb23
Allen & Kingery25
Humenik & Kingery26
Figure 10. The variation of contact angle between liquid iron and alumina substrate with temperature at oxygen potentials less than 10-13 Pa in the gas.
The general trend observed was that the contact angle values were nearly constant with respect to temperature. It is also seen that the values reported in this work are slightly higher than those obtained by other research groups. This is believed to be due to the extreme precaution taken in cleaning the argon gas in the present work. Through repeated analysis of the X-ray images, an error of the reported values was estimated to lie within . o4 The dynamic measurements of contact angles were carried out to monitor the change of contact angle as a function of time. The oxygen partial pressures imposed on the system were Pa and Pa. The X-ray images for the
experiment at 1823 K and oxygen partial pressure of Pa are shown in Figure 11. It is to be noted that the gas mixture was imposed onto the system at 0 second.
Figure 11. X-ray images from the sessile-drop experiment with molten iron on alumina substrate at
1823 K at different time intervals. The oxygen partial pressure of 3.010-3 Pa was imposed at zero time.
A sharp decrease in the contact angle is observed as oxygen is introduced into the system. Other research groups22-26,27,28,29,30 have made similar observations. A peculiar observation in the present work was that after the contact angle reached the minimum value, it started increasing again and the drop started moving laterally.
Cross sections of the used alumina crucible bottoms and the drops of iron from the experiments at 1823 K were subjected to microscopic as well as SEM analyses. In both cases, a product layer was identified between the alumina substrate and the iron drop. The photomicrographs of the cross sections of the alumina substrate under the experiments with and are shown in Figure 12 (a) and (b) respectively.
100 m (a) (b)
Figure 12 (a) and (b). Photomicrographs of the alumina substrate after the sessile-drop experiments at
1823 K and oxygen partial pressure of Pa and Pa, respectively. 3100.32
The micrograph from the experiment with Pa shows an average layer thickness of approximately 80 m and in the micrograph corresponding to an oxygen partial pressure of Pa, the average product layer thickness is approximately 30 m. This suggests that the penetration of the reaction product on the substrate was a function of the oxygen content of the metal, with the layer thickness increasing with increasing oxygen level. This is in agreement with the observations in the case of the alumina rod experiments.
EDS analysis of the product layers revealed that the layer had the following composition: 16 atom % Fe, 27 atom % Al and 57 atom % O. This would nearly correspond to the compound FeAl2O4, which is well in accordance with the thermodynamic analysis, which showed that at 1823 K hercynite would start forming at Pa. 5101
>OP 4.2.2 Iron on silica substrate In the case of iron on silica in purified argon gas, the contact angles were not found to change significantly with temperature, within the experimental temperature range and within the limits of the experimental errors. This behaviour is similar to the behaviour of iron on alumina substrate. However, in the present case, there were some difficulties in the measurements of the contact angles of the iron drops. At the experimental temperatures, the silica substrate was getting softened and the drop subsided slightly into the substrate. This was particularly serious at 1833 K. The error in the contact angle measurements, estimated from repeated analyses of the X-ray images was 2 at 1813 and 1823 K while it was higher at 1833 K, viz. 4.
In the second series of experiments, the measurements were carried out at an oxygen partial pressure of 1 Pa at 1823 and 1833 K. The X-ray images of the drops showing the change of drop shape with time at 1833 K are presented in Figure 13. The drop flattens as the atmosphere is changed to the gas mixture with higher oxygen partial pressure, thereby confirming that the contact angle decreases due to the introduction of the surface-active oxygen.
Figure 13. X-ray images of the sessile-drop experiment with molten iron on silica substrate at 1833 K
at different time intervals. The oxygen partial pressure of 1 Pa was imposed at zero time. 2105. Interestingly, the contact angle exhibits a tendency to increase after reaching a minimum point, which is clearly seen in the images in Figure 13. This is similar to the observations in the case of alumina substrate. At the end of the experiments, an ocular examination of the substrate and the drop revealed a thick layer of a slag phase at the base of the drop, surrounding it. The X-ray images of the iron drops in the experiment at 1823 K and Pa were similar to those obtained at 1833 K except that the decrease in the contact angle was not as pronounced. Similar to the alumina experiments, the drop started moving laterally just as the contact angle crossed the minimum value. Examination of the spot originally occupied by the drop revealed the formation of a small circular groove corresponding to the periphery of the drop in its initial position. The phenomenon is shown schematically in Figure 14. The slag layer formed at the drop-substrate interface was not as pronounced as in the earlier case.
iron drop groove
Figure 14. A schematic drawing of the silica substrate showing the groove formed at the periphery of
the iron drop in its initial position.
The SEM micrograph of the iron drop and the substrate, after the experiment at 1833 K is presented in Figure 15. The insert in the figure shows the location of the field of vision vis--vis the iron drop. The low contact angle between the drop and the substrate is quite evident in the figure. As mentioned earlier, a thick product layer is found to form around the drop. This evidently is the fayalite slag formed by reaction 4.
Figure 15. Photomicrograph of a section of the reacted drop and the silica substrate after the sessile-
drop experiments at 1833 and oxygen partial pressure, P Pa 2105.12
The atomic ratio of iron to silicon obtained by EDS analysis was close to 2, confirming the above observation. Higher magnification of Figure 15 clearly revealed the formation of dendrites to the right of the drop. These were found to be pure SiO2. The SEM micrographs of the drops at other oxygen partial pressures and temperatures were found to be similar. 4.2.3 Iron on mullite substrate The contact angle measurements of pure iron on mullite were carried out at 1823 and 1833 K for the same partial pressures of oxygen as before. For these experiments, an optical sessile-drop unit, available at the University of New South Wales, Australia was employed. The experimental details are presented in Supplement 4. Figure 16 shows the optical images of an iron drop at different time intervals. These images are from the experimental series with at 1823 K. As in the previous experiments, the gas mixture was introduced into the system at 0 second.
Figure 16. Optical images from the sessile-drop experiment with iron on mullite substrate at 1823 K.
The Pa was imposed at zero time. 3100.32
=OP Similar to the observations made in the experimental work with alumina and silica, the contact angle between the drop and the substrate decreases as the surface-active oxygen reached the metal. At the end of the experiments, the samples were quenched and the images from the run were analysed. Through repeated analysis of the images, the error in the contact angle measurement was estimated to be 6. After each experiment, the slag layer observed at the slag/substrate interface was examined in SEM. EDS analysis were carried out to determine the elements present. A micrograph from the SEM analysis for the experimental run at 1823 K and
Pa is shown in Figure 17. 2105.12
Figure 17. Photomicrograph of a section of the reacted drop and the mullite substrate after the sessile-
drop experiments at 1823 K and oxygen partial pressure, Pa. 2105.12
The insert in Figure 16 shows the location of the field of vision vis--vis the iron drop. It is seen that the iron drop has reacted with the substrate and has also sunk into it. A slag layer entrapped in the metal drop was observed and in this slag, small particles could be distinguished.
EDS mapping of the slag, Figure 18, shows that it consists of varying amounts of aluminium, silicon, iron and oxygen. The large particles in the slag were found to be alumina and in the periphery of these particles, there was a layer of hercynite.
Figure 18. EDS mapping of the slag formed during reaction between mullite substrate and molten iron
5. INDUSTRIAL REFRACTORY MATERIAL
In order to investigate the reaction with industrial aluminosilicate refractory material, sessile-drop experiments with industrial refractory substrate and pure iron as well as steel were carried out. The experimental procedure and the composition of the materials used are presented in Supplement 6. In the case of pure iron on refractory, the experimental work was carried out at 1873 K in an argon atmosphere and images from the experiment at two different time intervals are presented in Figure 19.
60 sec 120 sec
Figure 19. Images from the experiment with iron on industrial refractory in Ar atmosphere at different
time intervals. As seen, the contact angle does not vary much with time. The contact angle was calculated to be 111 at 1 min and 109 at 2 min. For the experiments conducted with refractory and steel (steel grade ORVAR 2M, Fe-0.37C-1.05Si-5.15Cr), the results were similar to the results for pure iron. The change in contact angle with time was not very pronounced as seen in Figure 20:
Figure 20. Images from the experiment with steel on industry refractory in Ar atmosphere at different time intervals.
The contact angles for this series were found to be approximately 106 and did not change much with time. Experiments were also carried out on an industrial scale. Samples were taken at the Uddeholm Tooling AB steel plant in Hagfors, Sweden. Details from the trials are presented in Supplement 6. Samples were taken from the ingot at different time
intervals. The samples were then analysed trough optical microscope and SEM/EDS analysis to see if a reaction product could be distinguished in the steel matrix. The analysis showed that no non-metallic particles were present.
6. MONTE CARLO SIMULATIONS
In the present work Monte Carlo simulations were carried out to understand the nature of alumina reaction at an atomic level. The main focus of the study was to investigate the interfacial phenomenon between graphite-alumina/ liquid iron. The system was chosen since simulations on the Fe-C-S system and carbon dissolution have been carried out earlier31,32,33 and a good understanding of the dissolution process has been obtained. It was felt that an extension of this work towards alumina-containing refractories would throw new light on the reaction mechanism. In this work, the interactions of alumina in refractory material and its effect on carbon dissolution have been carried out. 6.1 Theoretical model Two identical large blocks representing alumina-graphite refractory and molten iron were placed in contact with each other. This is schematically presented in Figure 21.
Figure 21. Schematic figure of the simulation arrangements
The alumina-graphite block consisted of randomly distributed alumina and graphite atoms. Molecular alumina was set as a unified group and occupied a single site. All sites on the block representing molten iron, were occupied by iron atoms. In the present simulations, the basal plane of the refractory block was placed in contact with iron as this plane has significantly more resistance to the interfacial reactions than the prismatic plane. The interactions between the atoms were assumed to be pair-wise as well as short-ranged and were restricted to the nearest neighbours. C-C bonding was assumed to be attractive as graphite is solid at the temperatures of interests. Al2O3-Fe bonding was assumed to be repulsive due to its non-wetting nature while Al2O3-Al2O3 and Al2O3-C bonding were also assumed to be attractive. The theoretical details and assumptions of the simulations and the Monte Carlo Algorithm are presented in Supplement 5. 6.2 Results Various process conditions such as alumina-graphite bonding strength, melt turbulence and wetting effect on carbon dissolution were investigated in the present work.
Different levels of bond strengths between alumina and graphite were used to simulate the possible effect various bonding agents might have on the refractory stability. In Figure 22, the equilibrium carbon concentration in the melt has been plotted as a function of the alumina-carbon bond strength.
Figure 22. Effect of the alumina-graphite bond strength
The bond strength of the alumina-graphite bonding increases with decreasing number on the X-axis. For refractory containing 80% C, the change in carbon dissolution is negligible. For the refractory with 30% C, however, there is a significant reduction in the carbon dissolution when the bond strength is increased. An explanation for this could be the dominating C-C bonding for the higher carbon refractory, making the change in alumina-graphite bonding less significant. As the wetting of iron on refractory is a factor that has an impact on the reaction rate, an attempt was made to incorporate the wetting behaviour in the present simulation. This was done by reversing the nature of the Fe-C interactions at the top surface of the solid in contact with the metal. In Figure 23, the results from these simulations are presented.
Figure 23. Effect of wetting behaviour on carbon dissolution
There are two sets presented in the graph; set A, which is the simulation without the wetting behaviour and set B, simulation with the wetting behaviour incorporated. It is seen that wetting is an important factor in considerably reducing the carbon dissolution from the alumina-graphite refractory.
In the alumina rod experiments, the thickness of the product layer was almost insignificant during the experiments where the dissolved oxygen level in the metal corresponded to the saturation solubility (0.2 wt% O) and almost no free FeO was present. On the other hand, at higher oxygen levels (with 1.9 wt % and 5 wt% oxygen in the melt), when the melt is expected to be in the Fe-FeO two-phase region, the corresponding corrosion reaction appears to be intense. This is in agreement with earlier observations1,2,34, with respect to the corrosive effect of FeO in the slag on the chemical attack on refractories. The thickness of the product layer at higher oxygen levels in the melt was found to increase with increasing reaction times as well as with increasing oxygen contents. The formation of the reaction layer was found to be diffusion controlled and under static conditions, the reaction between molten iron and dense alumina refractory was found to be topochemical, which is in conformity with the diffusion mechanism. In view of the few experimental points, an extensive kinetic analysis was not possible from the present results. According to the FeO-Al2O3 phase diagram, FeO is likely to react with alumina and form hercynite. The photomicrographs of the cross sections of the reacted alumina rods clearly show that a product layer was formed and that it strongly adhered to the alumina rod. According to the phase diagram, these two phases would be in equilibrium with each other and there is a slight solubility of FeAl2O4 in alumina, which could be an explanation of the strong adhesion of the layer to the substrate. The layer formation, along with the non-wetting conditions afterwards, that was observed in these experiments, is in conformity with the observations of Landefeld35. This would suggest that an effective way of protecting aluminabased refractories could be by forming a chemically non-wetting, adherent, product-layer on the refractory. The contact angle behaviour of liquid iron drop on alumina substrate obtained by the sessile-drop experiments could give some indication of the formation mechanism of hercynite. The change in contact angle with time at 1823 K and P Pa is presented in Figure 24.
When the gas mixture is imposed onto the system, there is an initial decrease in contact angle, which is likely to be due to the adsorption of oxygen on the surface of the metal drop. As the surface concentration of oxygen becomes high, diffusion of oxygen from surface to bulk becomes significant. Due to this, the surface concentration of oxygen cannot increase fast. Consequently, this leads to slow decrease of contact angle, and a pseudo steady state. Finally, when the droplet becomes saturated with oxygen corresponding to the imposed, it attains the equilibrium contact angle. The rapid decrease of contact angle after this point is probably due to change of dynamic contact angle to its equilibrium value. At this point there should be enough oxygen in the metal to form hercynite and the conditions change from wetting to non-wetting. This causes an imbalance in the forces acting on
the drop and the drop starts to move laterally. This phenomenon was clearly seen in the experimental work.
0 10 20 30 40 50 60 7060
Time [seconds] Figure 24. The change in contact angle with time for alumina at 1823 K and Pa 3100.3
=OP From the video images from the experiment at 1823 K and Pa, the force for the movement of the drop was estimated to be approximately 110
=OP-6 N. This was
found to be somewhat constant for a number of sequences except at the last stages, before the iron drop disappears out of the camera sight. The SEM-EDS analysis of the substrate in the present study shows that the composition of the product layers in Figures 12 (a) and (b) corresponds approximately to FeAl2O4. In view of the limited mutual solubility of hercynite and alumina, it can be surmised that the downward diffusion of FeAl2O4 through the Al2O3 substrate may be slow. In this case, the reaction gets stagnant and the contact surface would be covered completely by FeAl2O4 product layer. The experimental work on silica substrate showed the same tendency in contact angle change as in the case of alumina. In this case, a reaction product starts to form when the drop reaches the equilibrium oxygen content with respect to the gas phase. At this point there would be enough oxygen in the system for fayalite slag to form. There is a likelihood of a thin fayalite layer formation between the substrate and the drop, which would arrest the reaction. At this stage, the contact angle measured would most probably be between the iron drop with oxygen potential equal to that of the gas phase and the thin slag film on the silica substrate. Beyond this point, the contact angle showed a tendency to increase. This is also quite similar to the behaviour of the iron drop on the alumina surface. On the other hand, this increase could be measured in the case of the silica substrate as the drop was getting anchored to the substrate by the slag phase accumulated around it. This is clearly seen in Figure 25, which shows the change f contact angle of the iron drop on the silica substrate with time at 1833 K and Pa. The increase in the contact angle was accompanied by the tendency of the drop to move from its original position. This behaviour is quite analogous to the observations with the alumina substrate.
0 10 20 30 40 50 60
Time [seconds] Figure 25. The change in contact angle with time for silica at T=1833 for Pa. 2105.1
=OP In some of the experiments, there was a preferential corrosion observed along the periphery of the drop. This may be caused by the formation and evaporation of SiO, either due to direct decomposition of SiO2 substrate at the low oxygen potentials prevailing in the gas phase or by the reaction between silicon dissolved in the liquid metal and SiO2 substrate. Both the reactions would lead to the formation of SiO gas. These reactions would get dampened as the slag layer was formed around the bottom of the metal drop. Another plausible explanation is that the erosion is caused by Marangoni flow in the melt induced by differential surface tension due to concentration gradients. Analysis of the images from the sessile-drop experiments with iron on mullite substrate showed that the contact angle in purified argon atmosphere was 128, which is slightly lower that the contact angles obtained for alumina and silica. The change in contact angle with time for mullite and Pa at 1823 and 1873 K is presented in Figure 26.
0 10 20 30 40 50 60 70 80 90 100 110 120 130 14070
130 1823 K 1873 K
Time [seconds] Figure 26. The change in contact angle with time for mullite P at 1823 and 1873 K. 2105.1
=O It is seen that, similar to alumina and silica, there is a decrease in the contact angle when oxygen is introduced into the system and for the higher temperature, it
continues to decrease. For the lower temperature the contact angle seems to be stabilized for a while, but even in this experimental series, the contact angle decreased after some time. The slag formed during the reaction between mullite and molten iron would be different from the silica system. The thermodynamic analysis shows that when mullite and iron containing some amounts of oxygen start reacting, fayalite and hercynite will be formed. According to the ternary phase diagram presented in Figure 5, the mullite, fayalite and hercynite will start to dissolve into each other and form a ternary slag. At the experimental temperature, the ternary slag would consist of FeO-Al2O3-SiO2, the final composition being marked with an arrow in Figure 5. This slag will be in equilibrium with mullite and corundum. This is in agreement with the results of the SEM-EDS analyses. However, due to the kinetics of the reactions, there could still be particles of iron cordierite and hercynite as the reactions may not reach equilibrium. The composition of the slag would also change during cooling and low temperature phases could precipitate. This makes the interpretation of the results from the EDS analysis of the slag very complicated and difficult. The experimental work on mullite also showed that other factors, besides the composition of the substrate, would have an impact on the reaction mechanism. Factors like inhomogeneity, surface roughness and amounts of pores may also be of importance. The analysis of the porous mullite substrate revealed that, along with the surface reaction with the substrate, reactions were taking place downwards into the substrate, which could escalate the slag formation and corrosion of refractories. In the work on pure iron on industrial refractory, the results showed that the contact angle did not change much with time. This is expected, as the oxygen content in the atmosphere is low, which is similar to the conditions prevailing at the metal-refractory interface during casting. The contact angle was found to be approximately 110, which is lower than the values for alumina, silica and mullite in purified argon. One obvious reason is that the partial pressure of oxygen is lower in the purified argon gas compared to the un-treated gas. The other reason could be that less stable oxides present can dissolve into the molten iron and thus increase the oxygen content in the melt. However, the reactions were found to be very slow as the change in contact angle did not vary much with time. Similar observations were made for the experiments with industry refractory and steel. The contact angle was somewhat constant around 106 during the time interval of 3-1200 seconds. The slow reaction was also confirmed in the industrial trials that were carried out in this work. The samples from the outlet of the ingots showed that no reaction product had been formed. The Monte Carlo simulations in the present work showed that the bond strength between the different compounds in the refractory would play a significant role in the reaction rate, which in the present case is equal to the carbon dissolution. When the alumina-graphite bond strength increased, the dissolution of graphite decreased. This was more profound in the refractory containing higher amount of alumina as this would consist of more alumina-graphite bonding. The wettability of the substrate is also of importance for the reaction rate according to the simulations.
The present work is of great importance for the steel industry, especially for the steel plants targeting at the production of clean steel. The results show that the composition of the refractory plays a great role in corrosion of the furnace linings resulting in slag formation, which, in turn, can result in the formation of non-metallic inclusion in the steel matrix. The present work shows that silica, even though chemically bonded strongly in mullite, reacts with molten iron that contains some amounts of oxygen and forms a slag. The formation of a thin, dense, non-wetting hercynite layer between molten iron containing oxygen and alumina substrates shows a protective influence of the presence of higher alumina contents in the lining material, leading to less reaction with steel and thereby resulting in fewer non-metallic inclusions. A distinct possibility to increase the life of the furnace linings is to coat them with a non-wetting layer, for example, hercynite. This layer would act as a barrier between the refractory and the metal and it would prevent further reactions with the refractory. Of course, the economic gain in clean steel with these changes should be compared to the higher cost of refractory production.
The reaction between liquid iron containing oxygen and oxides were investigated through rod experiments as well as through sessile-drop experiments. In the latter, the oxygen in the melt was controlled by imposing an oxygen partial pressure in the gas phase above the drop using a suitable mixture of CO, CO2 and Ar gases. The sessile-drop images were followed both in the static as well as dynamic modes. In the case of alumina, the results showed the formation of a non-wetting product layer. Thermodynamic analysis of the Fe-O-Al system revealed that this layer should be FeAl2O4(s) under the prevailing experimental conditions. This was confirmed by EDS analysis of the layer. The thickness of the product layer was found to be a function of the reaction time and the oxygen content of the metal. In the case of silica and mullite refractories, the reactions resulted in the formation of a slag. With silica substrate, the slag was found to be fayalite ( . In the case of mullite, the slag phase formed contained alumina. The slag formation led to non-wetting conditions and the movement of the iron drop. Preferential corrosion of the silica refractory due to possible SiO evaporation or Marangoni convection was also observed in the present study. The factors influencing the corrosion of lining materials, apart from the chemical reactions, were oxygen content in the metal, porosity and surface roughness of the refractories.
Experiments with industrial refractories and steel as well as plant trials show that the contribution of runner refractories to the inclusion population of the final product is insignificant.
8. FUTURE WORK
The mullite experiments showed that the surface and the porosity of the substrate would play a roll in the corrosion and erosion of the substrate. It would be interesting to investigate this further. The amount of roughness, the shape of the roughness as well as the amount of pores and their shape are some parameters that should be looked into. Further, the impact of alloying elements and impurities like sulphur on the contact angle should be investigated. In the future, if the possibility of Monte Carlo simulation of a molten phase can be developed, the formation of slags and dispersion of solid phases in the same could be investigated at an atomic level to get a complete understanding of the reactions occurring.
9. REFERENCES 1 J. Bygdn, T. DebRoy and S. Seetharaman: Ironmaking and Steelmaking, 1994, vol. 21, p. 318-23. 2 P. Zhang and S. Seetharaman: J. Am. Ceram. Soc, 1994, vol. 77, p. 970-76. 3 N.L. Bowen and J.W. Greig, J. Am. Soc., 1924, 7, p. 242 4 I. Barin, Thermodynamical Data of Pure Substances, Part I and II, VCH, 1993. 5 J.C. Chan, C. B. Alcock and K.T. Jacob, Can. Metall. Quart.,1973, vol. 12, pp.439-43. 6 A. McLean and R.G: Ward, J. Iron Steel Inst, 1966, vol. 204, pp. 8-11. 7 F.D. Richardson, J.H.E. Jeffes and G. Withers, J. Iron Steel Inst,. 1950, vol. 162, pp. 213-45. 8 T.C. Pillay, J.DEntremont and J. Chipman, J. Am. Ceram. Soc., 1960, vol. 43, pp. 583-85.(Estimated
from R. Yamanaka, S. Koyama and M. Iwase, Metall. Met. Trans. B, 1991, vol. 22B, pp. 839) 9 Thermocalc, http://met.kth.se, Royal Institute of Technology. Stockholm, Sweden. 10 O. Knacke, O. Kubaschewski and K. Hesselmann, Thermo-chemical Properties of Inorganic
Substances, Heidelberg, Germany, Springer-Verlag, 1991. 11 E.T. Turkdogan, Physical Chemistry of High-Temp. Tech, Academic Press (1980), p.5 12 R.H. Rein and J. Chipman, Trans. TMS-AIME, 1965, vol. 223, pp. 415-25 (Estimated from R.
Yamanaka, S. Koyama and M. Iwase, Metall. Met. Trans. B, 1991, vol. 22B, pp. 839) 13 E.M. Levin, C.R. Robbins and H.F. McMurdie,. Phase Diagrams for Ceramists, M.K. Reser (ed.).
Ohio, USA, The American Ceramic Society, 1964, p.43 14 E.M. Levin, C.R. Robbins and H.F. McMurdie,. Phase Diagrams for Ceramists, M.K. Reser (ed.).
Ohio, USA, The American Ceramic Society, 1964, p. 696. 15 F.D. Richardson, Physical Chemistry of Melts in Metallurgy, vol. 2, Academic Press, London, 1974 16 R.N. Wenzel, Ind. Eng. Chem., 1936, vol. 28, no 8, pp. 988-94 17 Surface and Colloid Science, 1972, vol. 2, Ed. E. Matijevi, 18 K. Ogino A. Adach and K. Nogi, Tetsu-to-Hagan, 1973, vol. 59, pp. 1237-44 19 P. Kozakevitch, 1957 Symp. On Physical Chemistry of Steelmaking, MIT Press p.134 20 H. Gaye, L.D. Lucas, M. Olette and P.V. Riboud, Can. Metall, Q, 1984, vol. 23, pp. 179-191 21 A. Jakobsson, N. Nasu, J. Mangwiru, K.C. Mills and S. Seetharaman, Phil. Trans. R. Soc. Lond. A,
1998, vol. 356, pp. 995-1001. 22 A. Jakobsson, N.N. Viswanathan, Du Sichen and S. Seetharaman: Metall. Mater. Trans. B, 2000,
vol. 31B, p. 973-80. 23 I. Jimbo and A.W. Cramb: ISIJ. J. Int, 1992, vol. 32, p. 26-35. 24 A. Kasama, A. McLean, W.A Miller, Z. Morita and M.J. Ward: Cand. Metall. Q., 1983, vol. 22, pp.
9-17. 25 B.C. Allen and W.D. Kingery: J. Met., 1959, vol. 215, p. 30-37. 26 M. Humenik and W.D. Kingery: J. Amer. Ceram. Soc., 1954. vol. 37, p. 18-23. 27 F.A. Halden and W.D. Kingery: J. Phys. Chem., 1955, vol. 59, p. 557-59. 28 P. Kozakevitch and G. Urbain: Mem. Sci. Rev. Met., 1961, vol. 58, p. 517-34. 29 K. Ogino, K. Nogi and Y. Koshida: Tetsu-to-Hagan, 1973, vol. 59, p. 1380. 30 K. Hakashima, K. Takihira, K. Mori and N. Shinozaki: Mat. Trans JIM, 1992, vol. 33, p. 918.
31 V. Sahajwalla and R. Khanna, Metal. Mater. Trans. B, 2000, vol. 31B, pp. 1517-25 32 V. Sahajwalla and R. Khanna, Acta Mater. 1999, vol. 47 (3), pp. 793-800 33 V. Sahajwalla and R. Khanna, Scand. J. Metall. 2003, vol. 32, pp. 53-57 34 J. Bygdn, Trita-Mel rep. no. 131, Division of Theoretical Metallurgy, Royal Institute of
Technology, Stockholm, Sweden, 1993. 35 C.F. Landefeld: AFM Transaction, 1980, p. 507-14.
ABSTRACTACKNOWLEDGEMENTSSUPPLEMENTSTABLE OF CONTENTSSUMMARY1. INTRODUCTION2. THEORETICAL ASPECTS3. EXPERIMENTAL METHODS4. RESULTS5. INDUSTRIAL REFRACTORY MATERIAL6. MONTE CARLO SIMULATIONS7. DISCUSSION8. CONCLUSIONS8. FUTURE WORK9. REFERENCES